# Chapter 8 Phase Diagrams ### Chapter 8 Phase Diagrams

A

phase

in a material is a region that differ in its microstructure and or composition from another region

Al 2 CuMg Al H 2 O(solid, ice) in H 2 O (liquid)

2 phases

• homogeneous in crystal structure and atomic arrangement • have same chemical

and

physical properties throughout • have a definite

interface

and able to be mechanically separated from its surroundings

Chapter 8 in Smith & Hashemi Additional resources: Callister, chapter 9 and 10

Chapter 8 1

### Phase diagram and “degrees of freedom”

A

phase diagrams

is a type of graph used to show the

equilibrium

conditions between the thermodynamically-distinct phases; or to show what phases are present in the material system at various T, p, and compositions • “equilibrium” is important: phase diagrams are determined by using slow cooling conditions ⇒ no information about kinetics

Degree of freedom (or variance) F

is

the number

of variables (T, p, and composition) that can be changed independently without changing the phases of the system

Phase diagram of CO 2

Chapter 8 2

### 8.1 Phase Diagram of Water

3 phases: solid, liquid, vapour Triple point: 4.579 Torr (~603Pa), 0.0098

o C • • • Field – 1 phase Line – phase coexistence, 2 phases Triple point – 3 phases Chapter 8 3

### 8.2 Gibbs Phase Rule

Gibbs' phase rule describes the possible # of

degrees of freedom (F)

in a

closed system

at

equilibrium

, in terms of the number of separate

phases (P)

and the number of

chemical components (C)

in the system (derived from thermodynamic principles by Josiah W. Gibbs in the 1870s )

F + P = C + 2

F is # of degrees of freedom or variance P is # of phases

C is # of components Component

is the minimum # of species necessary to define the composition of the system

H 2 O C=1 (i) P=1, F=2; (ii) P=2, F=1; (iii) P=3, F=0

Chapter 8 4

### 8.3 How to construct phase diagrams? Cooling curves

Cooling curves

: • used to determine phase transition temperature • record T of material vs time, as it cools from its molten state through solidification and finally to RT (at a constant pressure!!!)

The cooling curve of a pure metal BC

:

plateaue

or

region of thermal arrest

; in this region material is in the form of solid and liquid phases

CD

: solidification is completed, T drops Chapter 8 5

### Cooling curve for pure iron @ 1atm

As T

: melted iron (liquid)

bcc Fe,

δ

(solid)

fcc Fe,

γ

(solid)

bcc Fe,

α

(RT)

Chapter 8 6

### 8.4 Binary systems (C = 2)

F + P = C + 2 = 4

F = 4 - P

Degrees of freedom (F): p, T, composition p T At p =

const (or T=const)

F = 3 - P

T composition 0 weight % of B 100%

100% A 100% B

1.

2.

Two components are completely

mixable

in liquid and solid phase (form a solid state solution), and don’t react chemically Two components (A and B) can form

stable compounds

or alloys (for example: A, A 2 B, A 3 B, B) Chapter 8 7

### Binary Isomorphous Alloy System (C=2)

Isomorphous:

Two elements are completely soluble in each other in solid and liquid state; substitutional solid state solution can be formed; single type of crystal str. exist

Reminder: Hume-Rothery rules

: (1) atoms have similar radii ; (2) both pure materials have same crystal structure; (3) similar electronegativity (otherwise may form a compound instead); (4) solute should have higher valence Example: Cu-Ni phase diagram (only for slow cooling conditions)

Liquidus line

: the line connecting Ts at which liquid starts to solidify under equilibrium conditions

Solidus

: the temperature at which the last of the liquid phase solidifies Between liquidus and solidus: P =2 Chapter 8 8

o

### C

P = 1 F = 3 – P = 2 P = 2 ; F = 3 – P = 1

• contains both liquid and solid phases ⇒ neither of these phases can have average composition 53 wt% Ni – 47 wt% Cu • draw

a tie line

at 1300 45% and solid phase w S o C ⇒ from the graph: composition of liquid phase w L = 58% at 1300 o C Chapter 8 = 9

### 8.5 The Lever Rule

The weight percentages of the phases in any 2 phase region can be calculated by using the

lever rule

Consider the binary equilibrium phase diagram of elements A and B that are completely soluble in each other Let

x

C o

Mass fraction of B

be the alloy composition of interest, its mass fraction of B (in A) is C ο Let

T

C L be the temperature of interest ⇒ at T alloy - mass fraction of B in liquid) and solid (C S

x

consists of a mixture of liquid (with - mass fraction of B in solid phase) 10

### Lever Rule (cont.)

Chapter 8 11

Q.:

A Cu-Ni alloy contains 47 wt % Cu and 53% of Ni and is at 1300 o C. Use Fig.8.5 and answer the following: A. What is the weight percent of Cu in the liquid and solid phases at this temperature?

B. What weight percent of this alloy is liquid and what weight percent is solid?

Chapter 8 12

### 8.6 Nonequilibrium Solidification of Alloys

⇐ constructed by using very slow cooling conditions Atomic diffusion is slow in solid state; as-cast microstructures show “core structures” caused by regions of different chemical composition Chapter 8

As-cast 70% Cu – 30% Ni alloy showing a cored structure

13

### Nonequilibrium Solidus

Solidification of a 70% Ni-30%Cu alloy

Fig. 8.9, Smith

Schematic microstructures at T2 and T4

Fig.8.10, Smith

• each core structure will have composition gradient α 1 α 7 • additional

homogenization

step is often required (annealing <T 7 ) Chapter 8 14

### 8.7 Binary Eutectic Alloy System

• • Components has

limited

solid solubility in each other Example: cooling 60%Pb – 40%Sn system

Liquid

⎯ ⎯ ⎯ ⎯ →

a

solid solution

+ b

solid solution This

eutectic

reaction ⇒ reaction is called an

invariant

occurs under equilibrium conditions at specific T and alloy composition F=0 at

eutectic

point Chapter 8 15

### Solubility Limit: Water-Sugar

• Changing T can change # of phases: path A to B . • Changing C o can change # of phases: path B to D 10 0 B (100,70) 1 phase D (100,90) 2 phases 80 60 40 20 L ( liquid solution i.e., syrup) L (liquid) + S (solid sugar) A (70, 20 ) 2 phases 0 0 2 0 4 0 6 0 70 8 0 Co=Composition (wt% sugar) Chapter 8 10 0 Adapted from Callister 16

# Binary Eutectic Alloy System

Figure 8.13, Smith

Chapter 8 17

Q: A lead-tin (Pb – Sn) alloy contains 64 wt % proeutectic ( α ) and 36% eutectic α+β 183 o C – ∆ T. Using Figure 8.13, calculate the average composition of this alloy.

at Chapter 8 18

### 8.8 Binary Peritectic Alloy System

The melting points of the two components are quite different A liquid phase reacts with the solid phase to form a new and different solid phase Liquid + α → β Chapter 8 19

Chapter 8 20

### 8.9 Binary monotectic systems

Monotectic reaction: a liquid phase transforms into a solid phase and another liquid phase L 1 → α + L 2 Chapter 8 21

### 8.10 Invariant Reactions

To summarize: 5 invariant reactions (F = 0) 1. Eutectic 2. Eutectoid 3. Peritectic 4. Peritectoid 5. Monotectic Liquid → α α → β + β + γ Liquid + α → β α + β → γ L 1 → α + L 2 The eutectic and eutectoid reactions are similar in that they both involve the decomposition of a single phase into two solid phases. The –

oid

suffix indicates that a solid, rather than liquid, phase is decomposing.

Chapter 8 22

8.11 Phase Diagrams with Intermediate Phases and Compounds

Terminal phase:

a solid solution of one component in another for which one boundary of the phase field is a pure component

Intermediate phase:

a phase whose composition range is between those of terminal phases Chapter 8 23

Ti-Si-O system • Experiment (700-1000 o C) Ti + SiO 2 → Ti 5 Si 3 and TiO y • At equilibrium the system will be in TiSi x – TiO y – SiO 2 three phase region (from calculations) • Ti 5 Si 3 – TiO – SiO 2 three phase region determined experimentally and remaining tie lines can be inferred Chapter 8 24

### 8.12 Ternary Phase Diagram

F + P = C + 2

For p = 1atm, T = const (isoterms) Cr-Fe-Ni alloy stainless steel Chapter 8 25

### Three and four component system

AB + AC = 2A + BC ∆ G = (2G A + G BC ) – (G AB + G AC ) If ∆ G <0, there is tie line between A and BC The remaining tie lines cannot cross A B AB BC AB + AC + AD = 3A + BCD ∆ G = (3G A + G BCd ) – (G AB + G AC + G AD ) AC C • • • Two phase equilibrium is represented by a tie line If ∆ G <0, there is a tie line between A and BCD; otherwise plane connects AB-AC-AD Chapter 8 26

### The Ti-Si-N-O quaternary phase diagram

• Entire phase diagram can be calculated by taking into account all possible combinations of reactions and products • 4 ternary diagrams of Ti-Si-N, Ti-N-O, Ti-Si-O and Si-N-O were evaluated • additional quaternary tie lines from TiN to SiO 2 and Si 2 N 2 O • stable metallization bilayer of TiN and TiSi 2 in contact with SiO 2 A.S.Bhansali,

et al., J.Appl.Phys.

68(3) (1990) 1043 Z.Chen,

et al., Phys.Stat.Sol.B

241(10) (2004) 2253 Chapter 8 27